Utilising Malaysian Fibre in Stone Mastic Asphalt as aReplacement of Imported Fibre
Ratnasamy Muniandy, Jeyan Vasudevan,Megat Johari Megat Mohd Noor &: Husaini OmarDepartment of Civil Engineeri~ Faculty of Engineering
Universiti Putra Malaysia43400 UPM, Serdang, Selang(ff
Stone Mastic Asphalt (SMA) technology is currently used in many countries. This is a gapgrade mix with a high percentage of coarse aggregates. As such there is a tendency forthe binder in the gap-graded mix to drain down during the hot weather that may causepremature failure of the mix. Various fibre types have been used successfully in SMA.However, the overall cost of the mix tends to be much higher than that in conventionalmix. This paper looks into the suitability of the Malaysian fibre for the use in SMA.
The fibre is analysed and compared with traditional European fibre that is commonlyused in SMA. Several experiments on the fibre have been done including Fibre DrainDown Test and Morphological analysis using the Scanning Electron Microscope (SEM).Besides this, chemical analysis was also carried out with a variation of cellulose content,particle size and Gas Chromatograph analysis. The result of the preliminary analysisshows that Malaysian fibre has the potential to replace the imported traditional fibre.
Keywords: Stone mastic asphalt, imported fibre and Malaysian fibre
In this current economic situation, the limited resource that is available should be usedat an optimum level to reduce the expenditure of the government in the laying of roads.Roads are the lifelines of a country. The sustainability, of this country's economydepends much on the land transportation system. According to roads branch (JKR1987) for the past ten years, an estimated RM3581 million has been spent to build roads,of which RM1560 million is spent on the maintenance of the existing roads, due to thefatigue cracking, rutting and stripping problem.
The above figure indicates that maintenance cost for road is very high. To cut downmaintenance cost and probably the overall cost of road laying and maintenance, analternative approach using the most advanced and durable pavement material such asStone Mastic Asphalt (SMA) has to be conducted.
Objective of Project Study
The main objective of this study is to analyse the suitability of the Malaysian fibre usedin Stone Mastic Asphalt. Several experiment or fibre analysis was conducted to determinethe characteristic of Malaysian fibre and its usage in SMA. This fibre study includesproduction, screening, pulping, chemical and mechanical analysis.
BACKGROUND ON STONE MASTIC ASPHALT
Stone Mastic Asphalt (SMA) is a gap-graded mix with a high coarse aggregate contentof 70-80%, binder content of 6.5-7.0% and filler contents of around 7-9%. Thepercentage of fibre that is required for SMA 0.3% and air voids of around 4%.
Ratnasamy Muniandy, Jeyan Vasudevan, Megat Johari Megat Mohd Noor & Husaini Omar
The skeletal formation of the coarse aggregate provides high resistance to deformation.Adding the fibres to the binder will prevent the asphalt from draining off duringstorage, transport and laying. Very soft binder may drain down easily. Bethune(1993)states that mastic fills the voids and retaining chips in position. It has an additionalstabilising effect, as well as providing the design air voids. The result is a highly durablerut resistant asphalt mix.
SMA can be used on all types of road and it is ideal for roads with heavy traffic. Itshigh binder content gives a longer life than conventional mixes. The second advantageis its coarse and open texture which generally provides high skid resistance at all speeds,as well as good drainage and fewer spray problems (Bethune 1993).
Analysis of FilJre Morphology by Scanning Electron Microscope
The Scanning Electron Microscope (SEM) output is shown in Plates1,2,3 and 4. Plate 2shows a thick presence of Malaysian fibre whilst Plate 1 shows otherwise. Plates 3 and 4shows the state of cellulose fibre after recovering from slight damage after mixing.
The imported traditional fibre is cellulose based fibre which is approximately 80%cellulose, whilst the Malaysian fibre is about 65% cellulose fibre. From Fig. 1, it can beseen that the percentage distribution of Holocellulose below 200/-tm is almost similar.From 200/-tm to 600/-tm a linear increment is observed. However, upon approaching apercentage distribution of 77% Holocellulose stage occur to the graph before reachingits ultimate condition from 600/-tm.
From Fig. 2, the percentage of alpha-cellulose below 200mm is constant but a gradualdecrement is noticeable. From 200/-tm to 600/-tm a linear decrement is observed.However, at 600/-tm the graph remains constant at 62.5% alpha-cellulose.
8700 \-+-------------:- \
r»"--\\-------------------~... \•t '\
\! ..i .....+------\
'~ ' -- .
".»"" ""_..-.."""'-------------_...._---.Fig. 2. % AlphaceUulose vs particle size
Ratnasamy Muniandy, Jeyan Vasudevan, Megat Johari Megat Mohd oor & Husaini Omar
The chemical analysis on Malaysian fibre by Liew and FRIM (1994) have been takeninto consideration. This analysis was conducted to monitor the presence of any deleterioussubstance that would react with asphalt. Table 1 and Table 2 show the chemicalcomposition and chemical properties of Malaysian fibre and imported fibre respectively.
Moisture ContentHot Water SolubleAlkali solubleAlcohol benzene soluble
Malaysian fibre (%)
Pyrolysis Gas Chromatography Analysis
Figure 3 shows the mixture for both asphalt with imported fibre and asphalt withMalaysian fibre. Results indicate that both peak at the same instance as plain asphalt forthe asphalt chemical component. Both the behaviour of imported and the Malaysianfibre display almost similar properties.
From this analysis it is clear that there are no deleterious components in the fibrethat may cause problems to the mix.
RESULTS OF THERMAL PULPING
After the grinding process, the particle was passed through a sieve size of 500flm priorto the pressurised thermal pulping. Plates 5 and 6 show the outcomes of pulping theMalaysian fibre and ilmported fibre. The fractional screening for Malaysian fibre andimported fibre is shown in Figs. 4 and 5 respectively. From the result obtain, it can beseen that the trend of particle distribution is almost the same for both Malaysian and theimported fibre but the sizes differ from 500flm for the Malaysian fibre and 50flm for theimported fibre.
Ramasamy Muniandy, Jeyan Vasudevan, Megat Johari Megat Mohd Noor & Husaini Omar
Fibre Drain Down Test
The drain down test is a traditional procedure to carry out sustainability of the Malaysianfibre against the imported fibre. From Fig. 6, it can be clearly seen that the Malaysianfibre is performing better than imported fibre. However, from Fig. 7, the performanceof the recovered fibre dropped slightly. It can be concluded that the performance ofMalaysian fibre was quite satisfactory.
MICROSCOPICAL EXAMINAnON I. O. • ,AVERAGE OF SIX SAMPLE :
C MICROSCOPiCAl EXAMINA-n-O-N1-.O. . '-"1~ LE AVERAGE OF SIX SAMPLE
~f'~~iPC 6.32 26.32 46.32
Fig. 4. Fractional screening for Malaysian fibre Fig. 5. Fractional screening for imported film
Imported fibre Malaysian fibre
Fig. 6. Comparison between imported & Malaysian fibre vs weight of oil passes
Based on the results obtained, the following conclusions were made. Firstly, the FibreMorphological analysis by Scanning Electron Microscope (SEM) and Fraction ScreeningAnalysis (sieve analysis) show that the pulped Malaysian fibre seemed to be thicker(below 500mm) compared to imported fibre (below 50mm). This condition of Malaysianfibre can be improved by further pulping.
Secondly, according to the results obtained from the chemical analysis, Malaysianfibre contains cellulose content of up to 65%, whilst imported fibre contain highercellulose of up to 80%. The advantage of the imported fibre is its soft structured naturein texture of alpha-cellulose, allowing easier expansion when heated up. This analysisalso shows that the expansion of the cellulose makes the asphalt more viscous and
....._.._-----_..._---Fig. 7. Comparison between recovered imported filne & recovered
Malaysian Filne vs weight of oil passes
provides the ability to retain the asphalt during the drain out process when temperatureincreases.
In the Fibre Drain Down test, by using motor oil, Malaysian fibre shows betterperformance than imported fibre within the allowable five minutes duration time ofdraining out period. There is however, a noticeable dripping of oil from Malaysian fibreindicating that it has yet to be stable. This may be assumed due to the thick presenceof Malaysian fibre. This assumption can be accepted when the Recovered Fibre DrainDown Test shows a stable drain out within the allowable duration. However, the resultsare still inferior compared to imported fibre. Even though the drain off rate is notcomparable to imported fibre but it is still acceptable because the performance of theMalaysian fibre is still within the given range, set by the European cellulose producer.
The main conclusion is that Malaysian fibre does perform comparably to importedfibre and could be an alternative supplement to replace imported fibre. However, morefinding is required to improve its performance.
BETHUNE J. and D. POTTER. 1993. Asphatic Innovations: Oversees Experience, Australian AsphaltPavement Association, Hawthorn, April 1993.
LlEw, Lio 'EL. 1994. Properties of medium density fibreboard made from oil palm (Elaesis Quineensis)trunk. B.Sc. Forestry (Wood Industry) Project Report. Faculty of Forestry, Universiti PertanianMalaysia, Serdang.
Tappi Testing Procedures. 1985. Atlanta: American National Standards Institute.
FRlM. 1994. Tests Data of Forest Research Institute Malaysia in Fibre From Oil Palm Fruit Bunches.Brochure of Sabutek (M) Sdn. Bhd. Kuala Lumpur, Malaysia.
NATIONAL AsPHALT PAVEMENT AssoCIATION (NAPA). 1996. Guidelines for Materials, Production, andPlacement of Stone Matrix Asphalt (SMA).
Asphalt Overlays for Highway and Street Rehabilitation. AI. Manual Series o. 17 (MS.17), SecondEdition, 1983.